Available online at www.sciencedirect.comhttp://dx.doi.org/0272-8842/& 20
nCorrespondinnCorrespondinE-mail addre(2015) 1444714457Ceramics International 41
www.elsevier.com/locate/ceramintTi/TiN/HA coating on Ti6Al4V for biomedical applications
E. Mohsenia, E. Zalnezhadb,n, A.R. Bushroaa,n, Abdel Magid Hamoudac, B.T. Gohd, G.H. Yoone
aCenter of Advanced Manufacturing and Material Processing, Department of Engineering, Faculty of Engineering, University of Malaya, 50603, MalaysiabDepartment of Mechanical Engineering, Hanyang University, 222 Wangsimni-ro, Seongdong-gu, Seoul 133-791, Republic of Korea
cMechanical and Industrial Engineering Department, College of Engineering, Qatar University, P.O. Box 2713, Doha, QatardLow Dimensional Materials Research Centre, Department of Physics, Faculty of Science, University of Malaya, 50603 Kuala Lumpur, Malaysia
eSchool of Mechanical Engineering, Hanyang University, Seoul, Republic of Korea
Received 22 May 2015; received in revised form 29 June 2015; accepted 14 July 2015Available online 21 July 2015Abstract
An unbalanced physical vapor deposition (PVD) magnetron sputtering technique was used to deposit a titanium/titanium nitride/hydroxyapatite(Ti/TiN/HA) multilayer coating on Ti6Al4V. The Taguchi optimization method with an orthogonal array of L9 was utilized to determine theoptimal conditions of coating for better surface integrity. The effects of the temperature, DC bias voltage, nitrogen flow rate, and DC power onthe adhesion strength, coefficient of friction, surface hardness, and surface roughness were investigated. In achieving the optimized coatingparameters, the signal to noise (S/N) response analysis method was implemented. Confirmation tests were carried out to demonstrate theimprovement using the best combination of parameters obtained from the optimization process. The surface hardness of the Ti/TiN coated anduncoated specimens was enhanced by 14% and 48%, respectively. The adhesion strength of the coating to the substrate, coefficient of friction,and surface roughness were improved by 5.1%, 43%, and 10.52%, respectively. Finally, hydroxyapatite was successfully deposited atop Ti/TiNcoated Ti6Al4V using a PVD sputtering technique to improve the biocompatibility of the substrate. The presence of Ti/TiN interfacial thinlayers between the HA layer and substrate enhanced the adhesion strength of the HA coating on the substrate by 44.57% compared to the HA-coated substrate without the interfacial layers.& 2015 Elsevier Ltd and Techna Group S.r.l. All rights reserved.
Keywords: Ti6Al4V; PVD magnetron sputtering; Ti/TiN coating; Hydroxyapatite; Mechanical properties1. Introduction
1.1. Titanium alloys for biomedical applications
Titanium (Ti) and its alloys (typically Ti6Al4V) arefrequently used in surgical implants and total joint replacementapplications (TJR) as a result of their high biocompatibility andmechanical properties. The high applicability of titanium alloysresults from their low density, corrosion resistance, and lowelastic modulus, which reduce stress shielding . However,other surgical alloys have demonstrated better adhesive and10.1016/j.ceramint.2015.07.08115 Elsevier Ltd and Techna Group S.r.l. All rights reserved.
g author. Tel.: 82 2 2222 0442; fax: 82 2 2222 3406.g author.ss: firstname.lastname@example.org (E. Zalnezhad).abrasive wear properties than titanium alloys . Subjectingan orthopedic device to relative sliding at the Ti alloy/metal orTi alloy/polyethylene interface results in fracture of the passi-vating surface oxide along with the creation of particulate metaland polyethylene debris and increased metal ion release.Accumulation of wear debris causes bone resorption, jeopardiz-ing the long-term stability of the prosthesis [9,10].Therefore, to improve the mechanical properties of Ti6Al
4V, a variety of surface modifications have been utilizedincluding nitrogen implantation and ultra-passivation of titanium. These methods have become a standard procedure for Tialloys. However, they are not guaranteed to provide adequatewear resistance of critical TJR components and long-termservice due to the rapid thinning of the r0.5 mm thickhardened layer [12,13]. The major constraints identified in the
Table 1Thin film coatings for tribological and surface integrity applications.
Coating technique Materials
Au, Ag, MCrAlYs, Cr, Mo
Sputtering SiO, SiO2, Cr, Mo, Au, TiC, TiN, Al2O3, WS2, MoS2,Si3N4
Ion plating Cr, Mo, TiC, TiN, Au, Ag, Si3N4
Table 2Chemical composition of Ti6Al4V.
Chemical composition of Ti6Al4V Alloy (wt%)
Al V Fe C O N Ti6.2 4.1 0.22 0.01 0.122 0.012 Bal.
E. Mohseni et al. / Ceramics International 41 (2015) 144471445714448aforementioned alloy are related to the tribological behavior,mainly in dry sliding wear due to its relatively low surfacehardness and significant ductility.
1.2. Hard tissue coating
The discipline of surface engineering allows improvement ofbulk material properties by applying micro and nanocoatings.Currently, there is high demand for hard thin film coatingmaterials such as titanium nitride (TiN) to enhance the mechan-ical properties of Ti alloys . A TiN coating layer has beenwidely used to enhance the hardness of different materials.However, it is difficult to control the properties of the film suchas the grain size, film thickness, and step coverage [18,19].Moreover, only limited data has been published regarding theinfluence of the TiN coating layer on various parameters such asthe scratch force, hardness, and roughness as well as the effect ofthe TiN coating layer microstructure of the deposited film [20,21].Investigation of this coating will demonstrate the possibility ofobtaining high strength, hardness, and simultaneously gooddecorative and protective surface properties . Surface mod-ifications have attracted more attention with new techniques suchas high power laser and vacuum processing. This fact isinteresting since these new techniques are highly comparablewith traditional surface modification techniques ranging frompainting and glazing to electroplating .
Based on a study by Mohseni et al. , titanium alloys such asTi6Al4V and a TiN coating layer are commonly used metallicmaterials for medical implants in orthopedic and dental applica-tions. However, there have been reports of inflammatory reactionsaround these implants as a result of the creation of an avascularfibrous tissue that encapsulated the implants. Thus, a hydroxyapa-tite layer coating can be deposited on the metal alloy to assist theosseointegration of these implants with surrounding tissues.Hydroxyapatite (HA: Ca10(PO4)6(OH)2) is a pure calcium phos-phate phase and a preferred biomaterial for both dental andorthopedics due to its favorable osteoconductive and bioactiveproperties .
Physical vapor deposition (PVD) is one of the most commonvacuum coating processes which has the ability to deposit the filmmaterial atom by atom on a substrate. The low process temperatureallows coating material to be deposited without reduction of thecorrosion resistance, loss of hardness, or distortion compared toother deposition techniques conducted at higher temperatures.Sputtering, ion plating, and thermal evaporation are three maintechniques for applying PVD coatings .
1.3. Magnetron sputtering PVD coating
Table 1 tabulates some of the vacuum coatings available toincrease the tribological properties of the sliding system. ThePVD magnetron sputter coating technique is an extremelyflexible coating technique that can be applied to coat virtuallyany material .
Good uniformity, better step coverage, strong adhesion ofthe coating to the substrate, and a small shadow effect are afew of the advantages of the sputtering technique. Goodcontrol of the effects of the parameters on the film character-istics including the film density, roughness, wear resistance,and adhesion strength is one important feature of the sputteringtechnique. Typical control parameters include the substratetemperature, process pressure, nitrogen flow rate, substrate biasvoltage, and process DC power .An optimization technique for the sputtering parameters is
necessary to achieve the best surface integrity. In this sense,the Taguchi method, which is an experimental design techni-que, was used to dramatically decrease the number of experi-ments by using orthogonal arrays and minimizing the out ofcontrol factors .In this work, optimization was performed to determine the
influence of surface modification of a Ti/TiN multilayercoating on Ti6Al4V to optimize the effects of the tempera-ture of the substrate, DC power, nitrogen flow rate, and DCbias voltage on the adhesion strength, surface hardness, androughness of the coating. Moreover, confirmation tests wereconducted to demonstrate the optimization. Finally, to increasethe biocompatibility of the substrate, an HA thin film wasdeposited on the existing Ti/TiN layers.2. Materials and methods
Ti6Al4V was utilized in this study. The compositionof the material characterized by EDX is given in Table 2.The Ti6Al4V samples were ground with 400 to 2000 SiCpaper and mirror finished with polycrystalline diamond sus-pended liquid (Buehler). The substrates were cleaned by anultrasonic machine using acetone for 20 min, followed byrinsing with disti